Role of Organic Counterion in Lead- and Tin-Based Two-Dimensional Semiconducting Iodide Perovskites and Application in Planar Solar Cells
Mao, Lingling; Tsai, Hsinhan; Nie, Wanyi; Ma, Lin; Im, Jino; Stoumpos, Constantinos C.; Malliakas, Christos D.; Hao, Feng; Wasielewski, Michael R.; Mohite, Aditya D.; Kanatzidis, Mercouri G.; Chemistry of Materials 28 (2016) 7781–; doi:10.1021/acs.chemmater.6b03054

data_4003314
_publ_section_title
;
 Role of Organic Counterion in Lead- and Tin-Based Two-Dimensional
 Semiconducting Iodide Perovskites and Application in Planar Solar Cells
;
_journal_issue                   21
_journal_name_full               'Chemistry of Materials'
_journal_page_first              7781
_journal_paper_doi               10.1021/acs.chemmater.6b03054
_journal_volume                  28
_journal_year                    2016
_chemical_formula_moiety         'I3 Sn, I, C5 H11 N3'
_chemical_formula_sum            'C5 H11 I4 N3 Sn'
_chemical_formula_weight         739.46
_space_group_crystal_system      monoclinic
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_atom_sites_solution_hydrogens   mixed
_atom_sites_solution_primary     direct
_cell_angle_alpha                90
_cell_angle_beta                 91.571(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   8.7411(4)
_cell_length_b                   20.0449(7)
_cell_length_c                   8.9845(3)
_cell_measurement_reflns_used    12328
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      32.65
_cell_measurement_theta_min      2.54
_cell_volume                     1573.62(10)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'XT (Sheldrick, 2015)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'image plate (34 cm diameter)'
_diffrn_detector_area_resol_mean 6.67
_diffrn_detector_type            STOE
_diffrn_measured_fraction_theta_full 0.984
_diffrn_measured_fraction_theta_max 0.979
_diffrn_measurement_details      ' 180 frames, detector distance = 100 mm'
_diffrn_measurement_device       '2-circle goniometer'
_diffrn_measurement_device_type  'STOE IPDS 2'
_diffrn_measurement_method       'rotation method'
_diffrn_radiation_collimation    '0.5 mm diameter, monocapillary'
_diffrn_radiation_monochromator  'plane graphite'
_diffrn_radiation_polarisn_norm  0
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0468
_diffrn_reflns_av_unetI/netI     0.0444
_diffrn_reflns_Laue_measured_fraction_full 0.984
_diffrn_reflns_Laue_measured_fraction_max 0.979
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       31
_diffrn_reflns_limit_k_min       -32
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            24323
_diffrn_reflns_point_group_measured_fraction_full 0.984
_diffrn_reflns_point_group_measured_fraction_max 0.979
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         34.986
_diffrn_reflns_theta_min         2.543
_diffrn_source
'sealed X-ray tube, 12 x 0.4 mm long-fine focus'
_diffrn_source_current           30
_diffrn_source_power             1.20
_diffrn_source_voltage           40
_exptl_absorpt_coefficient_mu    9.444
_exptl_absorpt_correction_T_max  0.7672
_exptl_absorpt_correction_T_min  0.4129
_exptl_absorpt_correction_type   integration
_exptl_absorpt_process_details   'STOE X-SHAPE'
_exptl_crystal_colour            'dark red'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   dark
_exptl_crystal_colour_primary    red
_exptl_crystal_density_diffrn    3.121
_exptl_crystal_description       plate
_exptl_crystal_F_000             1296
_exptl_crystal_preparation       'solution method'
_exptl_crystal_recrystallization_method 'precipitate after mixing'
_exptl_crystal_size_max          0.0470
_exptl_crystal_size_mid          0.0275
_exptl_crystal_size_min          0.0102
_refine_diff_density_max         0.908
_refine_diff_density_min         -1.737
_refine_diff_density_rms         0.216
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.096
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     123
_refine_ls_number_reflns         6770
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.096
_refine_ls_R_factor_all          0.1111
_refine_ls_R_factor_gt           0.0583
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0300P)^2^+5.0120P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0916
_refine_ls_wR_factor_ref         0.1087
_reflns_Friedel_coverage         0.000
_reflns_number_gt                4181
_reflns_number_total             6770
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            cm6b03054_si_002.cif
_cod_data_source_block           2
_cod_database_code               4003314